Reconstructive surgery for the repair of nose deformities is challenging . Nasal surgery involves autologous rib or septum cartilage grafts  and prosthetic devices  for reconstruction and reinforcement of the nasal skeleton. These conventional procedures are associated with donor site morbidity, limited tissue availability, and prosthesis related infection and extrusion . Although tissue engineering is a promising method for repair and reconstruction of cartilage defects [5- 7], engineering cartilage with a delicate three dimensional (3D) structure, such as human nose, remains a great challenge in this field. Since in 1997 Cao
One major reason leading to the failure of
To overcome these problems, two crucial issues should be addressed. First, the PGA-based scaffold should be prefabricated into the exact shape of human nose. Second, the mechanical strength of the above-mentioned scaffold should be further enhanced so that it can retain the pre-designed shape.
In order to meet these requirements, in the current study, a computer aided design and manufacturing (CAD/CAM) technique was employed to fabricate a set of negative molds, which was then used to press the PGA fibers into the pre-designed nose structure. Furthermore, the mechanical strength of the scaffold was enhanced by coating the PGA fibers with an optimized amount of PLA.
2. Materials and methods
2.1. Preparation of scaffolds with different PLA contents
10 mg of unwoven PGA fibers (provided by Dong Hua University, Shanghai, China) were compressed into a cylinder shape of 5mm in diameter and 2mm in thickness. A solution of 0.3 % PLA (Sigma, St. Louis, MO, USA) in dichloromethane was evenly dropped onto the PGA scaffold, dried in a 65 ºC oven, and weighed. The PLA mass ratio was calculated according to the formula: PLA%= (final mass-original mass)/final mass×100%. The above procedures were repeated until the predetermined PLA mass ratios of 0%, 10%, 20%, 30%, 40% and 50% were achieved. The scaffolds were examined by SEM (Philips XL-30, Amsterdam, Netherlands) .
2.2. Biocompatibility evaluation of the scaffolds
2.3. Mold fabrication by CAD/CAM
A patient’s normal nose was scanned by CT to obtain the geometric data (Figure 3). These data were further processed by a CAD system to generate both positive and negative of the normal nose, and the resultant data were input into a CAM system (Spectrum 510, Z Corporation) for the fabrication of the resin models by 3D printing. The negative mold was composed of two parts: the anterior part and the posterior part. (Figure 4A)
2.4. Fabrication of nose shaped scaffold
Two hundred milligrams of unwoven PGA fibers were pressed using the negative mold for over 12 hours. A solution of 0.3 % PLA (Sigma, St. Louis, MO, USA) in dichloromethane was evenly dropped onto the PGA scaffold, dried in a 65 ºC oven, weighed, and pressed again with the negative mold. This procedure was repeated until the final PLA mass ratio of 20% was reached. The edge of the scaffold was carefully trimmed according to the shape of the positive mold.
2.5. Statistical analysis
The differences of cell seeding efficiencies (n=6) among the six PLA content groups were analyzed using the Student’s t-test. A
3.1. SEM observation of the scaffolds with different PLA contents
PLA/PGA scaffold compositions were visualized under SEM. (Figure 1) The pure PGA scaffold (0% PLA added) appeared as a smooth fiber mesh. In PGA scaffolds supplemented with 10% PLA, the PLA coating can be seen connecting some fibers, particularly at nodes where PGA fibers cross. In the 20% PLA embedded scaffold, most mesh nodes visualized were covered with PLA. 30% PLA scaffold had not only most mesh nodes embedded in PLA, but also the PLA coating was seen covering small portions of the mesh itself, minimally obstructing the porosity of the fiber network. In the 40% PLA embedded scaffold, most of the mesh porosity is obscured by a PLA. In the 50% PLA scaffold, the mesh is almost completely obscured by a PLA sheet.
3.2. Evaluation of the biocompatibility of the scaffolds with different PLA contents
Cell seeding efficiencies were performed to evaluate the influence of PLA contents on cell compatibility of the scaffolds. The results showed that the increase in PLA content could lead to the reduction in the ability of the scaffolds to absorb the cell suspensions (Figure 2A). Quantitative analysis (Figure 2B) demonstrated that all the groups with PLA presented significantly lower cell seeding efficiencies compared to the group without PLA (p<0.05). If the acceptable cell adhesion rate is defined over 80%, these results indicate that 20% but not 30% is an acceptable PLA amount for preparing the scaffolds in terms of cell seeding efficiency.
3.3. Mold preparation and fabrication of the nose-shaped scaffold
Because good biocompatibility could be achieved in the scaffold with 20% PLA, this formulation was further used for the fabrication of the human nose shaped scaffold. In order to prepare the scaffold into a shape of normal nose, a set of negative molds was produced according to image of the normal nose (Figure 3). The resulting nose-shaped scaffold (Figure 4C) achieved a precise shape compared to its positive mold (Figure 4B). These results indicate that the mold produced by CAD/CAM technology is allowed to accurately fabricate a scaffold into a nose shape.
Despite the rapid progress in cartilage engineering,
To achieve this, a negative mold corresponding to the desired shape is required. CAD/CAM, as a novel technique, has been widely used for the fabrication of anatomically accurate 3D models [20- 23]. Particularly, this method can accurately perform complicated manipulations of the original 3D data, including Boolean operations, mirror imaging, and scaling [24- 26]. CAD/CAM technique was therefore used in the current study for the production of the negative mold for a human nose. Using this mold, PGA fibers were able to be accurately prepared into the nose-shaped scaffold.
The mechanical strength of PGA scaffold alone is not sufficient for the shape maintenance, and thus PLA coating was used to strengthen its mechanical properties as reported [10, 11, 27]. However, a high amount of PLA in the scaffold would negatively affect cartilage formation because of poor cell compatibility . Therefore, an appropriate PLA content in the scaffold is important for both shape maintenance and biocompatibility. In the current study, we evaluated the effects of six PLA contents on the scaffolds’ biocompatibility. According to the current results, although the mechanical strength of the scaffolds increased with increasing PLA content, 20% is an acceptable PLA amount for preparing the scaffolds in terms of cell seeding efficiency.
Finally, aided by CAD/CAM technique, the PGA fibers were prepared into the accurate shape of a human nose. Furthermore, by coating with PLA, the scaffold could obtain sufficient mechanical strength to retain the original shape. These results may provide useful information for future nose reconstructions by
In summary, this study established a method to precisely engineer a PGA/PLA scaffold with the shape of human nose. In future studies, we will also investigate the fate of these scaffolds after cell seeding, especially subcutaneous implantation in an immunocompetent animal model.
This research was supported by National Natural Science Foundation of China (81101438 and 81201476).
Anatomy, physiology, and general concepts in nasal reconstruction. Facial Plast Surg Clin North Am Bloom J. D Antunes M. B Becker D. G 2011 19 1 1 11
Cartilage grafting in nasal reconstruction. Facial Plast Surg Clin North Am Immerman S White W. M Constantinides M 2011 19 1 175 82
rd, Pearson JM. Nasal implants. Facial Plast Surg Clin North Am Romo T 2008 16 1 123 32vi.
Nasal tip ulceration from infection and extrusion of a nasal alloplastic implant. J Am Acad Dermatol Graham B. S Thiringer J. K Barrett T. L 2001Suppl): 362 4
Tissue engineering. Science Langer R Vacanti J. P 1993 260 5110 920 6
It is time to reconstruct human auricle more precisely and microinvasively. Plast Reconstr Surg Zhang L 2010e-156e.
Tissue Engineering of Musculoskeletal Tissue. In: Pallua N, Suschek C, eds. Tissue Engineering: From Lab to Clinic:Springer, Zhang L Spector M 2011
Transplantation of chondrocytes utilizing a polymer-cell construct to produce tissue-engineered cartilage in the shape of a human ear. Plast Reconstr Surg Cao Y Vacanti J. P Paige K. T Upton J Vacanti C. A 1997 100 2 297 302discussion 303-4.
In vitro tissue engineering to generate a human-sized auricle and nasal tip. Laryngoscope Kamil S. H Kojima K Vacanti M. P Bonassar L. J Vacanti C. A Eavey R. D 2003 113 1 90 4
Repair of articular cartilage defect in non-weight bearing areas using adipose derived stem cells loaded polyglycolic acid mesh. Biomaterials Cui L Wu Y Cen L Zhou H Yin S Liu G Liu W Cao Y 2009 30 14 2683 93
Di Cesare PE. Scaffolds for articular cartilage repair. Ann Biomed Eng Frenkel S. R 2004 32 1 26 34
Mini-review: Mechanical factors affecting cartilage regeneration in vitro. Biotechnol Bioeng Heath C. A Magari S. R 1996 50 4 430 7
Comparison of scaffolds and culture conditions for tissue engineering of the knee meniscus. Tissue Eng Aufderheide A. C Athanasiou K. A 2005
Characterization of polylactic acid-polyglycolic acid composites for cartilage tissue engineering. Tissue Eng Moran J. M Pazzano D Bonassar L. J 2003 9 1 63 70
The impact of low levels of collagen IX and pyridinoline on the mechanical properties of in vitro engineered cartilage. Biomaterials Yan D Zhou G Zhou X Liu W Zhang W. J Luo X Zhang L Jiang T Cui L Cao Y 2009 30 5 814 21
Biodegradable synthetic polymers for tissue engineering. Eur Cell Mater Gunatillake P. A Adhikari R 2003 5 1 16discussion 16.
Engineering smooth muscle tissue with a predefined structure. J Biomed Mater Res Kim B. S Mooney D. J 1998 41 2 322 32
In vitro engineering of human ear-shaped cartilage assisted with CAD/CAM technology. Biomaterials Liu Y Zhang L Zhou G Li Q Liu W Yu Z Luo X Jiang T Zhang W Cao Y 2010 31 8 2176 83
Comparison of three types of chondrocytes in collagen scaffolds for cartilage tissue engineering. Biomed Mater Zhang L Spector M 2009
Stereolithography in oral and maxillofacial operation planning. Int J Oral Maxillofac Surg Bill J. S Reuther J. F Dittmann W Kubler N Meier J. L Pistner H Wittenberg G 1995Pt 2):98-103.
CAD/CAM ear model and virtual construction of the mold. J Prosthet Dent Ciocca L Mingucci R Gassino G Scotti R 2007 98 5 339 43
An opinion survey of reported benefits from the use of stereolithographic models. J Oral Maxillofac Surg Erickson D. M Chance D Schmitt S Mathis J 1999 57 9 1040 3
Rapid development of auricular prosthesis using CAD and rapid prototyping technologies. Int J Oral Maxillofac Surg Subburaj K Nair C Rajesh S Meshram S. M Ravi B 2007 36 10 938 43
Al Mardini MErcoli C,Graser GN. A technique to produce a mirror-image wax pattern of an ear using rapid prototyping technology. J Prosthet Dent 2005 94 2 195 8
CAD-CAM generated ear cast by means of a laser scanner and rapid prototyping machine. J Prosthet Dent Ciocca L Scotti R 2004 92 6 591 5
Fabrication of an auricular prosthesis using computed tomography and rapid prototyping technique. J Craniofac Surg Karayazgan-saracoglu B Gunay Y Atay A 2009 20 4 1169 72
The design of scaffolds for use in tissue engineering. Part I. Traditional factors. Tissue Eng Yang S Leong K. F Du Z Chua C. K 2001 7 6 679 89